Multiple phase and dielectric transitions on a novel multi-sensitive [TPrA][M(dca)3] (M: Fe2+, Co2+ and Ni2+) hybrid inorganic-organic perovskite family
J. M. Bermudez-Garcia; M. Sanchez-Andujar; S. Yanez-Vilar; S. Castro-Garcia; R. Artiaga; J. Lopez-Beceiro; L. Botana; A. Alegria; M. A. Senaris-Rodriguez; Journal of Materials Chemistry C 4 (2016) 4889–4898; doi:10.1039/C6TC00723F

data_7234783
_publ_section_title
;
 Multiple phase and dielectric transitions on a novel multi-sensitive
 [TPrA][M(dca)3] (M: Fe2+, Co2+ and Ni2+) hybrid inorganic-organic
 perovskite family
;
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              4889
_journal_page_last               4898
_journal_paper_doi               10.1039/C6TC00723F
_journal_volume                  4
_journal_year                    2016
_chemical_formula_sum            'C18 N10 Ni'
_chemical_formula_weight         414.95
_space_group_crystal_system      tetragonal
_space_group_IT_number           140
_space_group_name_Hall           '-I 4 2c'
_space_group_name_H-M_alt        'I 4/m c m'
_atom_sites_solution_hydrogens   .
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 90.000(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            4
_cell_length_a                   11.390(5)
_cell_length_b                   11.390(5)
_cell_length_c                   17.301(5)
_cell_measurement_temperature    368(2)
_cell_volume                     2244.5(15)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      368(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0480
_diffrn_reflns_av_unetI/netI     0.0141
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            27474
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.172
_diffrn_reflns_theta_min         2.354
_exptl_absorpt_coefficient_mu    0.889
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2008/1 (Bruker AXS Inc.)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.228
_exptl_crystal_description       prism
_exptl_crystal_F_000             824
_exptl_crystal_size_max          0.61
_exptl_crystal_size_mid          0.51
_exptl_crystal_size_min          0.46
_exptl_transmission_factor_max   0.667
_exptl_transmission_factor_min   0.584
_refine_diff_density_max         0.418
_refine_diff_density_min         -0.208
_refine_diff_density_rms         0.060
_refine_ls_extinction_coef       0.092(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     67
_refine_ls_number_reflns         699
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.154
_refine_ls_R_factor_all          0.0480
_refine_ls_R_factor_gt           0.0402
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0689P)^2^+2.4585P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1157
_refine_ls_wR_factor_ref         0.1282
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                568
_reflns_number_total             699
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6tc00723f2.cif
_cod_data_source_block           '[TPA][Ni(dca)3]368K'
_cod_original_cell_volume        2244(2)
_cod_database_code               7234783
_shelx_res_checksum              8980
_shelx_hkl_checksum              4616